 states which are energetically far from the $E_F$ are not contribute much on $C_Q$. The density of state near the Fermi level for a given material can be tune by means of an efficient chemical modification of the system using external ad-atoms or creating defects. This is also an effective way to control the type and concentration of charge carriers in the system. The electronic Energy levels of the parent material may also be modified/shift in these process. The change in electronic structure depends on dopant type, concentration and doped position in the sublattice. In this study we have considered atoms from different groups in periodic table with an increasing order of electronegativity such as K$<$ Na$<$ Al$<$ P$<$ N$<$ Cl, to functionalize the graphene. The stable adsorption position on graphene was estimated by placing ad-atoms in different possible adsorption sites and comparing the optimized total energies. The hollow position was found to be the most favourable position for ad-atoms like K, Na, Al, bridge position for P, N and top position for Cl ad-atoms respectively. The optimized structure of functionalized graphene with different adsorption positions are shown in Fig. \[FG-Adatom Optimized structure\]. The stability of the functionalized structure was investigated by estimating average adsorption energy $E_{ad}$ for ad-atoms using $$E_{ad} = \frac{1}{n}[E_{tot} - E_{gr} -nE_{at}]$$ where $E_{tot}$ is the total energy of the functionalized graphene unit cell, $E_{gr}$ is the total energy of pristine graphene in the same unit cell, $E_{at}$ is the per atom energy of the ad-atom and $n$ represents the number of ad-atoms present in the unit cell. The adsorption energies for different ad-atoms are listed in the Table. \[table1\]. Our calculation shows that the adsorption of N on pristine graphene surface is most favourable compare to other ad-atoms. However relatively large adsorption energies for P, Cl and Al clearly indicate that these can be easily adsorb on the pristine graphene surface. The ad-atoms are adsorbs on graphene at a distances varying from 1.5 Å to 3.3 Å from the surface. Interestingly, the planar structure of graphene is not much disturbed with these adsorptions. However a very small change in the C-C bond lengths (order of 0
states which are energetically far from the $ E_F$ are not contribute much on $ C_Q$. The density of department of state near the Fermi degree for a given material can be tune by means of an effective chemical modification of the system using external ad - atom or creating defects. This is besides an effective direction to control the character and concentration of charge carriers in the system. The electronic Energy level of the parent material may also be modified / shift in these process. The variety in electronic structure depends on dopant type, assiduity and doped position in the sublattice. In this study we have considered atoms from unlike groups in periodic board with an increasing order of electronegativity such as K$<$ Na$<$ Al$<$ P$<$ N$<$ Cl, to functionalize the graphene. The stable adsorption stead on graphene was estimated by placing ad - atoms in different possible adsorption sites and comparing the optimized total energies. The hollow position was found to be the most favourable position for ad - atoms like K, Na, Al, bridge military position for P, N and top position for Cl ad - atom respectively. The optimize structure of functionalized graphene with different adsorption positions are indicate in Fig. \[FG - Adatom Optimized structure\ ]. The stability of the functionalized structure was investigated by estimate average adsorption energy $ E_{ad}$ for ad - atoms using $ $ E_{ad } = \frac{1}{n}[E_{tot } - E_{gr } -nE_{at}]$$ where $ E_{tot}$ is the total energy of the functionalized graphene whole cell, $ E_{gr}$ is the total energy of pristine graphene in the same unit of measurement cell, $ E_{at}$ is the per atom department of energy of the ad - atom and $ n$ map the number of ad - atoms present in the unit cell. The adsorption department of energy for different ad - atoms are listed in the Table. \[table1\ ]. Our calculation usher that the adsorption of N on pristine graphene surface is most favourable compare to early ad - atoms. However relatively large adsorption energies for P, Cl and Al clearly bespeak that these can be easily adsorb on the pristine graphene open. The ad - atoms are adsorbs on graphene at a distance varying from 1.5 Å   to 3.3 Å   from the airfoil. Interestingly, the planar structure of graphene is not much disturbed with these adsorptions. However a very small variety in the C - C bond lengths (orderliness of 0
 stwtes which are energeticxlly far from tkw $E_F$ ace not dontribuge much on $C_Q$. The density of srate bear the Fermi level fur a givej materiql cen be tune by meehs of ak effjgient rhemical modifigation of tve system usinc dxcernal ad-atoms or creating defects. Tris is sldo an effectivg way eo ckntrol the type and concentration kf charje carriers in yhe system. The electronic Fnerhy levels of the pwrent materual iqy also be mudified/shift in these krocess. The change in electronic strueture depenes on gopant type, concvntration and doped pmsition in the sublatbice. Mn tyis study we have convidered atoms from differend yroups in periodic tavlw witv an incfwaskng ocded of epecvronegativify such as J$<$ Na$<$ Al$<$ P$<$ N$<$ Cl, to finsnoonalize the graphqnq. The stable adsorption position on grakhene was estimated by placibg ad-atoms in differejt possibje adsorption sites and comparing the optimized tmtal xndrgncf. Rhf hollow position was found to be the most fadkutanle position for ad-atoms lile K, Ga, Al, bridge kositiou fkr P, N and top posltion fjr Cl ad-atoms wesprctively. The optimized struxture of funbtiobalized graphene wnth differenc adsotption positions are shown in Fig. \[FG-Adatom Ootimized agructure\]. The stacilpty mf the functionalized strusture was invzstigatea by estimwting averwge adsorption energy $E_{af}$ for ag-atoms usijg $$E_{ad} = \frac{1}{n}[E_{tot} - E_{gr} -nE_{at}]$$ whecx $E_{tot}$ is the tmtan energy of tme functionalizqd graphene unnt cell, $Z_{gr}$ is the total energy of pristinq graphene in jhe same unit cell, $E_{ae}$ is the per atuo energy of thr ad-atom cud $n$ reprwsents the number pf xs-atoms present nu uhw unit cell. Thr aasowpnioi enewcies for difxerevt xc-atomr are listeb kn tne Table. \[table1\]. Our cdlcumation shows that yhc adsorptuon of N on pristine braphene surface id mosv favonrable coipare to other ad-atoms. However relativepy jarge adsorpeion energies fox P, Cl and Al clearly indicate that thesx can be easily adsorb in the pristine grakheke surface. Tie ad-aeoms are ddsorbs on graphene qt a distances vavying from 1.5 Å to 3.3 Å from tge surxace. Lnterestingly, the planar structure of graphene is not much disturbed with these adsorptions. Howrver d rerv small chaigx in the C-C bond kengths (order of 0
states which are energetically far from the not much on The density of for given material can tune by means an efficient chemical modification of the using external ad-atoms or creating defects. This is also an effective way to the type and concentration of charge carriers in the system. The electronic Energy of parent may be modified/shift in these process. The change in electronic structure depends on dopant type, concentration and position in the sublattice. In this study we considered atoms from different in periodic table with an order electronegativity such K$<$ Al$<$ N$<$ Cl, to the graphene. The stable adsorption position on graphene was estimated by placing ad-atoms in different possible adsorption and comparing total energies. hollow was to be the position for ad-atoms like K, Na, for P, N and top position for Cl respectively. The structure of functionalized graphene with different positions are shown in Fig. \[FG-Adatom Optimized structure\]. stability of the functionalized structure was investigated by estimating average adsorption energy $E_{ad}$ for ad-atoms = \frac{1}{n}[E_{tot} - E_{gr} where $E_{tot}$ is total of functionalized unit cell, is the total energy of pristine graphene in the same unit $E_{at}$ is the per atom energy of the ad-atom and the of ad-atoms present the unit cell. The energies different ad-atoms are listed Table. Our the of on pristine graphene surface most favourable compare to other However relatively large adsorption Al clearly indicate that these can be easily on the pristine graphene surface. The ad-atoms adsorbs on graphene at a distances varying from 1.5 Å to 3.3 from the the planar structure of graphene is not much with these adsorptions. However very small change in the C-C bond lengths (order 0
 states which are energeticalLy far from tHe $E_F$ aRe nOt cOnTribUte mUch on $C_Q$. The densITy of State near the Fermi level For a gIvEN matERiAl can Be tune bY MeANS of An EfFicIeNT cHemicAl mOdificaTion of the sYstEm Using externaL Ad-Atoms or creAtiNg defects. ThiS is Also an EfFecTIve waY to ContrOl the tYPe and cOncentratIoN Of charGE carrieRS In The sYstem. The electroniC enERgy levels of the Parent MaTErIAL maY alSo be modifiEd/Shift IN these pROcESS. the CHange in electrOnic structuRE dePends oN dOpaNT type, cOncenTrATioN and doped poSitiOn in the suBlattiCE. In this STudy we hAve conSidEreD atoMS fRoM diFfERenT GrOupS In pEriodic tAbLe With aN incREASIng oRdeR of eLectrOnegativity suCh aS K$<$ Na$<$ aL$<$ P$<$ N$<$ cl, to fUnctiOnalIzE the gRaphenE. The sTaBle adsorption poSitiOn on graphEne WaS esTiMated BY placiNg aD-atOms in diFferent POssIbLE ADsOrption sites and comPaRINg The optimIzed toTAl EnERgies. The HoLloW posITIon waS fouND tO be the moSt favoURaBlE positiOn For ad-aToMs lIke k, Na, Al, BRidgE positIon for P, N And toP Position for Cl aD-Atoms respectiVElY. tHe OPtimIzeD structure oF funCTionAlizED gRapHEne wiTh difFeREnT Adsorption positions ArE shown In Fig. \[fG-Adatom OptimIzed structURE\]. the stabiLity OF tHE functionalizeD struCture was inVEstigateD by esTimating Average adSORption enErgY $E_{aD}$ foR ad-ATOmS using $$E_{ad} = \frac{1}{N}[e_{Tot} - E_{Gr} -NE_{at}]$$ wheRe $E_{Tot}$ is thE toTal EneRgy Of The functiOnalized GrApHeNe UniT cell, $e_{Gr}$ is the tOtAl eNeRgy Of priSTine grAphenE in tHe SaME unIt cell, $E_{AT}$ iS THe peR aToM eneRgy Of The ad-Atom ANd $n$ RepreseNts the numBer OF ad-aToMs Present In the unit cell. thE adsorptioN eNerGies foR DIfferent Ad-atoms are listed in the TaBLe. \[table1\]. our CalcuLatiOn shows thAt tHe adsoRptIOn of N oN pristIne grApHenE SUrfacE IS mOst FaVourable coMPAre To othEr Ad-atOms. HoweVer relatively large ADsoRption energieS foR P, Cl AND AL clEArLY inDiCAte THAt these can be easIly adsorb oN tHE pRistine graPHenE sUrface. THe ad-atoMs are ADsorbs oN graphene At a distanCeS varYINg fRom 1.5 Å to 3.3 Å froM the surfAce. IntereSTinglY, ThE planAr sTructuRe Of gRapheNe is noT MucH distUrbed wItH these AdsorPtIons. HoweVer a very small change in thE C-C bonD lengThs (Order of 0
 states which are energeti cally farfromthe  $E _F $ ar e no t contribute m u ch o n $C_Q$. The density o f sta te near th e Fer mi leve l  f o r  agi ve n m at e ri al ca n b e tuneby means o f a nefficient ch e mi cal modifi cat ion of the s yst em usi ng  ex t ernal  ad -atom s or c r eating  defects.  T h is isa lso ane f fe ctiv e way to controlt he type and conce ntrati on of c har gecarriers i nthe s y stem. T h ee l e ctr o nic Energy le vels of the par ent ma te ria l  may a lso b em odi fied/shiftin t hese proc ess. T h e chang e  in ele ctroni c s tru ctur e  d ep end so n d o pa ntt ype , concen tr at ion a nd d o p e d  pos iti on i n the  sublattice.Inthis stu dy we  have  con si dered  atoms  from  d ifferent groups  inperiodictab le  wi th  an i n creasi ngord er of e lectron e gat iv i t y  s uch as K$<$ Na$<$Al $ < $P$<$ N$< $ Cl,t ofu n ctionali ze  th e gr a p hene.  The st able ads orptio n  p os ition o ngraphe ne  wa s e stima t ed b y plac ing ad-a tomsi n different po s sible adsorpt i on s it e s an d c omparing th e op t imiz ed t o ta l e n ergie s. Th eh ol l ow position was fou nd  to be  themost favourab le positio n f or ad-at omsl ik e  K, Na, Al, br idgeposition f o r P, N a nd to p positi on for Cl a d-atomsres pec tiv ely . Th e optimized s t r uctu re  of fun cti onalize d g rap hen e w it h differe nt adsor pt io npo sit ionsa re shown  i n F ig . \ [FG-A d atom O ptimi zedst ru c tur e\]. Th e  s t a bili ty  o f th e f un ction aliz e d s tructur e was inv est i gate dby  estima ting averagead sorption e ne rgy  $E_{a d } $ for ad -atoms using $$E_{ad} = \frac{1 }{n }[E_{ tot}  - E_{gr}  -n E_{at} ]$$ where$E_{to t}$ i sthe t otale n er gyof  the funct i o nal izedgr aphe ne unit  cell, $E_{gr}$ is the  total energy  of  pri s t in e g r ap h ene  i n  th e same unit cell,  $E_{at}$is th e per atom ene rg y of th e ad-at om an d  $n$ re presentsthe numbe rof a d - ato ms present  in theunit cell .  Thea ds orpti onenergi es  fo r dif ferent ad- atoms  are l is ted in  theTa ble. \[t able1\]. Our calculatio n show s tha t t he adsorp tio n  of  N on pri stin e graphene  su rfa ce is  mo s t fav oura b le  co m pareto o t her ad-at o ms . H o w ev er relative l y lar ge ad sor p tion e nerg ies for P, Cl and Al clearly ind icat e tha t t h eseca n be easily ad sor bo n  the pri st ine graphen e surfac e. The a d-atom s areadsorbs o ng raphen e at  adistances  va ry i ng from  1 .5 Å to 3 .3 Å  f rom th e surf a ce.I n terestingly, the  plan a r  stru c tur e ofgr aphenei s no t much dis turbed with  these  ads orpti ons. Ho we ver aver ysmall chan g e in theC-C b ond len gt hs ( ord er of0
 states_which are_energetically far from the_$E_F$ are_not_contribute much_on_$C_Q$. The density_of state near_the Fermi level for_a given material_can_be tune by means of an efficient chemical modification of the system using external_ad-atoms_or creating_defects._This_is also an effective way_to control the type and_concentration of_charge carriers in the system. The electronic Energy_levels_of the parent_material may also be modified/shift in these process. The_change in electronic structure depends on_dopant type, concentration_and_doped_position in the sublattice._In this study we have considered_atoms from different groups in periodic_table with an increasing order of electronegativity_such as K$<$ Na$<$ Al$<$ P$<$_N$<$ Cl, to functionalize the_graphene. The_stable adsorption position on graphene_was estimated by_placing ad-atoms_in different possible_adsorption sites and comparing the optimized_total energies. The_hollow position was found to be_the_most favourable position_for_ad-atoms_like K,_Na, Al, bridge_position_for P,_N_and top position for Cl ad-atoms_respectively._The optimized structure of functionalized graphene with_different adsorption positions are_shown_in Fig. \[FG-Adatom Optimized_structure\]. The stability of the_functionalized structure was investigated by estimating_average adsorption_energy $E_{ad}$_for ad-atoms using $$E_{ad} = \frac{1}{n}[E_{tot} - E_{gr} -nE_{at}]$$ where $E_{tot}$_is the total energy of the_functionalized graphene unit cell,_$E_{gr}$ is_the_total energy of_pristine_graphene in_the same unit cell, $E_{at}$ is the_per atom_energy of the ad-atom and $n$_represents the number of_ad-atoms_present in the unit cell. The_adsorption energies for different ad-atoms are_listed in the Table. \[table1\]._Our_calculation_shows that the adsorption of_N on pristine graphene surface is_most favourable compare_to other ad-atoms. However relatively large adsorption_energies_for P, Cl and Al clearly_indicate_that these can be easily adsorb_on_the_pristine graphene surface. The ad-atoms_are adsorbs on graphene at a_distances varying from 1.5 Å to 3.3 Å from the surface._Interestingly, the planar_structure of graphene is not_much_disturbed_with these adsorptions. However a very small change in the_C-C bond_lengths (order of_0